• date post

06-Apr-2020
• Category

## Documents

• view

1

0

Embed Size (px)

### Transcript of Title Here NdFeB for High Temperature Motor Applications · PDF file NdFeB are 1.05 •...

• 1 © Arnold Magnetic Technologies

Title Here

Author Venue Date

NdFeB for High Temperature

Motor Applications

Steve Constantinides with Dale Gulick

SMMA Fall Technical Conference November 3-5, 2004

• © 2004 Arnold, Magnetic Technologies 2

• To understand what happens to a magnet at elevated temperature, or in the presence of a reverse magnetic field or a combination, it is necessary to understand the basics of magnetism.

• The first section will cover some of the more important magnetic characteristics.

2 © Arnold Magnetic Technologies

Topics

• Magnet Basics

• Temperature Effects

• Demagnetization Stress

• Combined Effects

• © 2004 Arnold, Magnetic Technologies 3

3 © Arnold Magnetic Technologies

Applied Field

Hysteresis Loop

+H Oersteds

(A/m)

-H Oersteds

(A/m)

+B Gauss (Tesla)

-B Gauss (Tesla)

ea su

re d

In du

ct io

n

• We describe the hysteresis “loop” on a grid with X and Y axes except that we call the horizontal axis the “H” axis measured in Oersteds (or kA/m); the vertical axis is the “B” axis measured in Gauss (or Tesla, T).

• The H axis represents the magnitude of an externally applied field to the magnet material. The B axis represents the magnetic output either of the magnet or the combination of the magnet and the applied field.

• Note: in air, one Gauss = one Oersted. The distinction is that Oersted refers to applied field and Gauss to the measured, resultant (induced) field.

• The grid is divided into quadrants. The first quadrant is often referred to as the magnetizing quadrant, and the second is often referred to as the demagnetizing quadrant.

• © 2004 Arnold, Magnetic Technologies 4

4 © Arnold Magnetic Technologies

Free space induction (slope = perm = 1.0)

Observable induction (normal)

Applied field

In du

ce d

fie ld

(I nd

uc tio

n)

Magnetic material induction (intrinsic)

Bs

• As an external field is applied to our sample, the “B” measurement increases corresponding to the applied field.

• As the external field increases, the magnet starts to contribute to the output. That is, a field is induced in the magnet.

• When the magnet is saturated, the increase in B is once again equal to the increase in H.

• © 2004 Arnold, Magnetic Technologies 5

5 © Arnold Magnetic Technologies

1st Quadrant: Relaxation of Applied Field

Applied field

In du

ce d

fie ld

(I nd

uc tio

n)

Note flux density does not follow original magnetization.

Observable induction (normal)

Magnetic material induction (intrinsic)

Br

All external field removed at this point

Free space induction (slope = perm = 1.0)

• As the H field is reduced, B also falls. • The value of B where H=0 is called residual induction, Br. • Two curves may be seen here: the normal (green) and the intrinsic (blue). • The normal curve represents the measured, combined B value of both the applied field and

that contributed by the magnetic material. • The intrinsic curve is the calculated output due only to the magnet and is obtained by

subtracting H from B.

• © 2004 Arnold, Magnetic Technologies 6

6 © Arnold Magnetic Technologies

Applied field

In du

ce d

fie ld

(I nd

uc tio

n)

Magnetic material induction (intrinsic)

Observable induction (normal)

HcHci

Net magnetization

is lost.

Free space induction (slope = perm = 1.0)

Free space induction (slope = perm = 1.0)

• If the external field is now applied in the opposite direction, the value of B will become smaller. At first, only a small reduction is noted.

• When there is sudden and substantial reduction in the magnet’s field compared to the change in applied demagnetizing field, we say that the we have exceeded the second quadrant knee of the material.

• There are two very important points here. • Hc or HcB, coercive force: When the magnet reaches this condition, it has no observable

(external) field because the applied field H (= Hc) is balanced out by the flux M of the magnet material. Because they are in the opposite direction, the net observable induction B is equal to zero.

• Hci or HcJ, intrinsic coercivity: As the applied H is increased, past the “knee” of the intrinsic curve, the net magnetization of the material, M, reaches zero. This is the Hci, or intrinsic coercive force.

• © 2004 Arnold, Magnetic Technologies 7

7 © Arnold Magnetic Technologies

Hysteresis Loop - 3rd and 4th Quadrants

Applied field

In du

ce d

fie ld

(I nd

uc tio

n)

Free space induction (slope = perm = 1.0)

• The applied field can be increased until the magnet’s field has been fully reversed, in the third quadrant.

• If we then remove the applied field, the hysteresis loop returns to H=0 and with a negative value for Br.

• Applying a positive field, we move through the fourth quadrant and intercept the initial curve at saturation in the first quadrant.

• The third and fourth quadrants are essentially the same as the first and second quadrants, except they are in the opposite polarity.

• The entire curve is the “hysteresis loop”.

• © 2004 Arnold, Magnetic Technologies 8

8 © Arnold Magnetic Technologies

Hysteresis Loop - All Quadrants

Applied field

In du

ce d

fie ld

(I nd

uc tio

n)

Hc

Br

Normal curve

Intrinic curve

Hci

• This chart displays the two types of hysteresis loops for a permanent magnet material: the Normal Curve and the Intrinsic Curve.

• At every point the two hysteresis loops will differ by the value of H: (B = Bi + H). In the first quadrant B = Bi +(+ H) or B=Bi +H. In the second quadrant B=Bi+(-H) or B=Bi-H. If you have one curve (e.g., B vs. H), you can calculate the other (e.g., Bi vs. H)

• The hysteresis curve shown is typical of a “straight line demagnetization” material, a.k.a., “square loop” material. “Straight line” refers to the normal curve’s linear response in the second quadrant. ”Square loop” describes the knee shape of the intrinsic curve.

• This behavior is typical of ferrite and rare-earth magnets (NdFeB and SmCo). For Alnico and Iron Chrome Cobalt, the intrinsic curve is very similar to the normal curve. They are so similar on these alloys that the Hci is approximately the same as the Hc.

• Bonded rare earth magnets exhibit a hysteresis loop somewhat less than “straight line.”

• © 2004 Arnold, Magnetic Technologies 9

• At this point we can use the hysteresis curves (Fig 1) and the DC magnetizing curves (Fig 2) to demonstrate the difference between the soft magnetic materials and the hard magnetic materials.

• Intrinsic Coercivity (Hci) is most often used to delineate between “hard” and “soft” materials. Most “soft” magnetic materials exhibit Hci < 25 Oersted (See Fig 1), i.e., the ease with which they can be magnetized. If a small applied field suffices to produce saturation, the material is said to be magnetically soft. (See Fig 2). If a large field is required, as represented by curve “c,” the material is said to be magnetically hard. Materials having properties between “hard” and “soft” materials are occasionally referred to as “semi-hard” magnetic materials (curve “b”).

• For a hard magnetic material, the area inside the hysteresis curves (Fig 1) should be large because it represents the amount of useful magnetic energy that can be made available to do work. For soft magnetic material, it represents undesirable “core loss” and the area should be minimized.

9 © Arnold Magnetic Technologies

Soft vs. Hard (Permanent) Magnetic Materials

H

B

Hci

Soft

Hard

25

O e

Figure 1: Hysteresis Curve

Bsat

a

500-XX,000)

Figure 2: Magnetizing Curve

a: soft

b: semi-hard

c: hard

B

H

• © 2004 Arnold, Magnetic Technologies 10

• When the operating point on the normal curve is known, the energy product of the magnet may be calculated. This is calculated by multiplying the Bd value by the Hd value. Energy = Bd x Hd , e.g., the energy products for points 1 and 2 are Hd1 x Bd1 or Hd2 x Bd2

• This calculates the rectangular area under the normal curve between the origin and the operating point. Common units obtained are Gauss-Oersteds and are typically referred to in Mega Gauss Oersteds (MGOe in cgs, and Joules/cubic meter in SI).

• Maximum Energy is found by locating a single point on the Normal curve where the product of Bd x Hd is greater than at any other point. For “Straight Line” materials this point is at approximately Bd = 1.1 Hd

• BHm